182 
DE. A. MATTHIESSEN ON THE SPECIEIC GEAVITY OF ALLOYS. 
Table II. (continued.) 
Tin-Gold Series (determined by Dr. M. Holzmajs’^n). 
Alloy. 
Mean of 
Calculated specific 
gravity, from 
volume. 
Ratio of volumes, 
V+Vj 
V 
Specific gravity 
found. 
T. 
7-441 
22-9 
7-446 
1-0007 
SnJo Au 
7-801 
22-8 
7-786 
0-981 
Sfljg Au 
8-118 
22-4 
8-092 
0-9968 
Snj 2 Au 
8-470 
23-1 
8-452 
0-9979 
Sug Au 
8-931 
25-6 
8-951 
1-0023 
Siig Au 
9-405 
23-7 
9-407 
1-0002 
Sug Au 
9-715 
22-4 
9-743 
1-0029 
Sn^ Au 
10-168 
23-7 
10-206 
1-0037 
Sug Au 
10-794 
23-6 
10-885 
1-0084 
Sug Au 
11-833 
14-6 
11-978 
1-0022 
Sn Au 
14-244 
14-2 
14-028 
0-9848 
Sn Aug 
16-367 
15-4 
15-913 
0-9722 
Cadmium-Bismuth Series (determined by A. Matthiessen). 
Cdg Bi 
9-079 
13-1 
9-067 
0-9987 
Cd^ Bi 
9-195 
15-5 
9-181 
0-9985 
Cdg Bi 
9-388 
15-0 
9-380 
0-9991 
Cd Bi 
9-554 
13-4 
9-550 
0-9996 
Cd Big 
9-669 
14-8 
9-668 
0-9999 
Cd Bi^ 
9-737 
14-7 
9-740 
1-0003 
Cd Big 
9-766 
15-4 
9-766 
1-0000 
Cadmium-Lead Series (determined by Dr. M. Holzmann). 
CdgPb 
9-160 
13-7 
9-173 
1-0014 
Cd^Fb 
9-353 
12-0 
9-364 
1-0012 
CdgPb 
9-755 
14-7 
9-780 
1-0026 
Cd Pb 
10-246 
11-7 
10-246 
1-0000 
Cd Pbg 
10-656 
13-4 
10-663 
1-0006 
Cd Pb4 
10-950 
9-2 
10-966 
1-0015 
Cd Pbg 
11-044 
14-8 
11-088 
1-0039 
Bismuth-Silver Series (determined by Dr. M. Holzmann). 
^hoo 
9-802 
23-5 
9-825 
1-0023 
Biso Ag 
9-813 
23-6 
9-829 
1-0016 
Bl24 Ag 
9-820 
23-3 
9-836 
1-0016 
Bii 2 Ag 
9-836 
21-8 
9-848 
1-0012 
Bis Ag 
9-859 
21-0 
9-871 
1-0012 
Bh Ag 
9-899 
15-2 
9-893 
0-9994 
Bis Ag 
9-966 
14-9 
9-949 
0-9983 
Bi Ag 
10-068 
15-6 
10-034 
0-9966 
Bi Agg 
10-197 
13-2 
10-141 
0-9945 
Bi Ag4 
10-323 
15-1 
10-249 
0-9928 
